Presentation on theme: "Injection Molding Fiber Orientation, Property Predictions, and Failure Analysis Presented by Robert Sherman Senior CAE Analyst, RTP Company."— Presentation transcript:
Injection Molding Fiber Orientation, Property Predictions, and Failure Analysis Presented by Robert Sherman Senior CAE Analyst, RTP Company
o Source of Fiber Orientation o What Causes it o New AMI 2012 Analysis Features o RSC Factor & Its Effects o Modulus (& Stress) Predictions o Without RSC o Various RSC Factors o Improved Stress Predictions What Well TRY to Cover
o Injection molding products are being utilized in increasingly structural applications o To date, analysis has consisted of quasi- isotropic analysis o Quasi-isotropic analysis CANNOT optimize orthotropic materials properly o Orthotropic analysis requires failure analysis and strength allowables o What can be utilized?? ? Structural Composites from the Injection Molding Process
o Sensible approach to the problem: Composite laminate analysis o Injection molded materials can be treated like continuous fiber composites o Problem : Infinite number of orientations! o Systematic approach for evaluation is needed in order to prevent unexpected failures o Linear material approach initially Structural Composites from the Injection Molding Process
o Two primary forces o High shear rate & velocity gradient through part thickness o Extensional forces in flow front expansion and contraction o Fiber orientation is history dependent – effects are cumulative as polymer flows from gate to end-of-flow What Causes Fiber Orientation ?
o Shearing forces in outer laminates o Expansional/contractional forces in middle laminates o Changing flow directions during fill/pack o Orientation behavior is sum of the cumulative effects Fiber Orientation
o Fill Preview (real-time fill prediction solver) o Inventor Fusion Interface for model simplification o Transient cooling analysis o Venting analysis o Long fiber orientation capability (ARD model) o Short fiber orientation improvements (RSC model) Autodesk® Moldflow® Insight New Analysis Features
o All fiber orientation predictions previously were fully developed steady state orientation o Reality – orientation takes time to fully develop o RSC factor introduced to control the rate of development of orientation o Problem: limited validation to date (Delphi; 2 PBT materials) o Take cup half-full approach Reduced Strain Closure (RSC) Factor
o Qualitative validation can utilize microscopy o Made quantitative with shape recognition software o Micro tomography analysis (Skyscan) o Simpler (cheaper) method of validation needed for number of materials needing validation o Utilize tensile modulus predictions and measurements as first cut validation o Later confirm with flexural stiffness verification How Can We Validate Fiber Orientation ?
What does RSC Factor Do?
Look at Molded Tensile Bars First
Flow Direction Modulus (RSC=1.00) t = 3.05 mm (0.120 in)
Modulus Transverse to Flow (RSC=1.00) t = 3.05 mm (0.120 in)
Flow Direction Modulus (RSC=0.15) t = 3.05 mm (0.120 in)
Modulus Transverse to Flow (RSC=0.15) t = 3.05 mm (0.120 in)
Flow Direction Modulus t = 6.35 mm (0.250 in)
Modulus Transverse to Flow t = 6.35 mm (0.250 in)
Laminate Stress Analysis
o RSC factor clearly seems to improve the fiber orientation predictions o More correlation is needed (flexural modulus) o Other possible influencing factors may need improvement o Relook at fiber A/R utilized (usually too low) o Other boundary conditions o More materials to determine factors influencing RSC Summary
Presented by Robert Sherman Senior CAE Analyst, RTP Company Thank You!